Home > Documents > TIE-29 Refractive Index and Dispersion - Schott AG · • Refractive Index Measurement 1....

# TIE-29 Refractive Index and Dispersion - Schott AG · • Refractive Index Measurement 1....

Date post: 02-Jan-2020
Category:
View: 26 times
12
Introduction The most important property of optical glass is the refractive index and its dispersion behavior. This technical information gives an overview of the following topics: Dispersion – Principal Dispersion – Secondary Spectrum – Sellmeier Dispersion Equation Temperature Dependence of Refractive Index Inﬂuence of the Fine Annealing Process on the Refractive Index and Abbe number Tolerances Refractive Index Measurement 1. Refractive Index If light enters a non-absorbing homogeneous material reﬂection and refraction occurs at the boundary surface. The refractive index n is given by the ratio of the velocity of light in vacuum c to that of the medium v n = c v (1) The refractive index data given in the data sheets are measured relative to the refractive index measured in air. The refractive index of air is very close to 1. 1. Refractive Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .1 2. Wavelenght Dependence of Refractive Index: Dispersion . . . . . . . . . . . . . . . . . . . . . . 2 3. Temperature Dependence of Refractive Index . . . . . 6 4. Influence of the Fine Annealing Process on the Refractive Index and Abbe number . . . . . . . . . . . . . . . 7 5. Tolerances . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9 6. Refractive Index Measurement . . . . . . . . . . . . . . . . . . . 11 7. Literature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .12 Refractive Index and Dispersion Practically speaking the refractive index is a measure for the strength of deﬂection occurring at the boundary surface due to the refraction of the light beam. The equation describing the amount of deﬂection is called Snell’s law: n 1 · sin(a 1 ) = n 2 · sin(a 2 ) (2) The refractive index is a function of the wavelength. The most common characteristic quantity for characterization of an optical glass is the refractive index n in the middle range of the visible spectrum. This principal refractive index is usually denoted as n d – the refractive index at the wavelength 587.56 nm or in many cases as n e at the wavelength 546.07 nm. Technical Information Advanced Optics TIE-29 Version February 2016 1
Transcript

Introduction

The most important property of optical glass is the refractive index and its dispersion behavior. This technical information gives an overview of the following topics:• Dispersion – Principal Dispersion – Secondary Spectrum – Sellmeier Dispersion Equation• Temperature Dependence of Refractive Index• Influence of the Fine Annealing Process on the

Refractive Index and Abbe number • Tolerances• Refractive Index Measurement

1. Refractive Index

If light enters a non-absorbing homogeneous material reflection and refraction occurs at the boundary surface. The refractive index n is given by the ratio of the velocity of light in vacuum c to that of the medium v

n = cv

(1)

The refractive index data given in the data sheets are measured relative to the refractive index measured in air. The refractive index of air is very close to 1.

1. Refractive Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1

2. Wavelenght Dependence of Refractive Index: Dispersion . . . . . . . . . . . . . . . . . . . . . . 2

3. Temperature Dependence of Refractive Index . . . . . 6

4. Influence of the Fine Annealing Process on the Refractive Index and Abbe number . . . . . . . . . . . . . . . 7

5. Tolerances . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9

6. Refractive Index Measurement . . . . . . . . . . . . . . . . . . . 11

7. Literature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12

Refractive Index and Dispersion

Practically speaking the refractive index is a measure for the strength of deflection occurring at the boundary surface due to the refraction of the light beam. The equation describing the amount of deflection is called Snell’s law:

n1 · sin(a1) = n2 · sin(a2) (2)

The refractive index is a function of the wavelength. The most common characteristic quantity for characterization of an optical glass is the refractive index n in the middle range of the visible spectrum. This principal refractive index is usually denoted as nd – the refractive index at the wavelength 587.56 nm or in many cases as ne at the wavelength 546.07 nm.

TIE-29

Version February 2016

1

2

2. Wavelength Dependence of Refractive Index: Dispersion

The dispersion is a measure of the change of the refractive index with wavelength. Dispersion can be explained by apply-ing the electromagnetic theory to the molecular structure of matter. If an electromagnetic wave impinges on an atom or a molecule the bound charges vibrate at the frequency of the incident wave.

The bound charges have resonance frequency at a certain wavelength. A plot of the refractive index as a function of the wavelength for fused silica can be seen in figure 1. It can be seen that in the main spectral transmission region the refractive index increases towards shorter wavelength. Additionally the dotted line shows the absorption constant as a function of the wavelength.

2.1 Principal DispersionThe difference (nF – nC) is called the principal dispersion. nF and nC are the refractive indices at the 486.13 nm and 656.27 nm wavelength.The most common characterization of the dispersion of optical glasses is the Abbe number. The Abbe number is defined as

nd = (nd – 1)/(nF – nC) (3)

Sometimes the Abbe number is defined according to the e line as

ne = (ne – 1)/(nF' – nC') (4)

Back to index➜ ➜

Refractive Index and Dispersion

Fig. 1: Measured optical constants of fused silica (SiO2 glass) [1].

Traditionally optical glasses in the range of nd > 50 are called crown glasses, the other ones as flint glasses.

Glasses having a low refractive index in general also have a low dispersion behavior e. g. a high Abbe number. Glasses having a high refractive index have a high dispersion behavior and a low Abbe number.

Wavelength λ/µm

Ref

ract

ive

Ind

ex n

(λ)

Ab

sorp

tio

n C

on

stan

t k

(λ)

3.5

3.0

2.5

2.0

1.5

1.0

0.5

0

101

100

10–1

10–2

10–3

10–4

10–1 100 101

nk

TIE-29

3

2.2 Secondary SpectrumThe characterization of optical glass through refractive index and Abbe number alone is insufficient for high quality optical systems. A more accurate description of the glass properties is achievable with the aid of the relative partial dispersions.

The relative partial dispersion Px,y for the wavelengths x and y is defined by the equation:

Px,y = (nx – ny)/(nF – nC) (5)

As Abbe demonstrated, the following linear relationship will approximately apply to the majority of glasses, the so-called ”normal glasses”

Px,y ≈ axy + bxy · nd (6)

axy and bxy are specific constants for the given relative partial dispersion.In order to correct the secondary spectrum (i. e. color correc-tion for more than two wavelengths) glasses are required which do not conform to this rule. Therefore glass types having deviating partial dispersion from Abbe’s empirical rule are especially interesting.

As a measure of the deviation of the partial dispersion from Abbe’s rule the ordinate difference ΔP is introduced. Instead of relation (6) the following generally valid equation is used:

Px,y = axy + bxy · nd + ΔPx,y (7)

The term ΔPx,y therefore quantitatively describes a dispersion behavior that deviates from that of the ”normal glasses”.

The deviations ΔPx,y from the ”normal lines” are listed for the following five relative partial dispersions for each glass type in the data sheets.

PC,t = (nC – nt)/(nF – nC) PC,s = (nC – ns)/(nF – nC) PF,e = (nF – ne)/(nF – nC) (8) Pg,F = (ng – nF)/(nF – nC) Pi,g = (ni – ng)/(nF – nC)

The position of the normal lines is determined based on value pairs of the glass types K7 and F2. The explicit formulas for the deviations ΔPx,y of the above-mentioned five relative partial dis-persions are:

ΔPC,t = (nC – nt)/(nF – nC) – (0.5450 + 0.004743 · nd) ΔPC,s = (nC – ns)/(nF – nC) – (0.4029 + 0.002331 · nd) ΔPF,e = (nF – ne)/(nF – nC) – (0.4884 – 0.000526 · nd) (9) ΔPg,F = (ng – nF)/(nF – nC) – (0.6438 – 0.001682 · nd) ΔPi,g = (ni – ng)/(nF – nC) – (1.7241 – 0.008382 · nd)

Figure 2 shows the Pg,F versus the Abbe number nd diagram.

The relative partial dispersions listed in the catalog were cal culated from refractive indices to 6 decimal places. The dispersion formula (10) can be used to interpolate additional unlisted refractive indices and relative partial dispersions (see chapter 2.3).

Back to index➜ ➜

Refractive Index and Dispersion

TIE-29

4

0.6590100 80 70 60 50 40 30 20

90100 80 70 60 50 40 30 20

10

10

0.63

0.62

0.61

0.60

0.59

0.58

0.57

0.56

0.55

0.54

0.53

0.52

0.51

0.65

0.63

0.64 0.64

0.62

0.61

0.60

0.59

0.58

0.57

0.56

0.55

0.54

0.53

0.52

0.51

P g,F =

ng

– n

F

nF –

nC

P g,F =

ng

– n

F

nF –

nC

νd

νd

Febr

uary

201

6

P-SK57Q1

F2

N-KZFS8*

N-KZFS5*

LAFN7

SF56A

SF6

N-LAF21N-LAF35

N-LASF44*

N-LASF31AP-LASF47

N-LAF34N-LAK10

N-LAF2N-LASF41

N-LAF33

N-KZFS4*

N-KZFS2*

N-KZFS11*

F5N-LASF40

N-LAK21

N-LAK14N-LAK9*

N-LAK34

N-LAK8

K10

N-LAK22

N-SK2*N-SK4

K7

N-BAK4

N-BALF4

N-KF9

N-SSK5

N-SSK8

N-FK58

N-BALF5

N-SSK2N-LAK12N-BAK1

P-SK57

N-LAK7

N-SK16

N-SK14N-SK5

N-SK11N-ZK7

N-BAK2

N-K5

N-BK10N-FK5*

N-PSK3N-BK7*

N-PSK53A*

LF5

N-BASF64

N-BASF2

N-SF5*

N-SF1

SF10N-SF8

N-SF15

P-SF8

N-SF10

N-SF4

SF57*N-SF6

N-SF11

N-SF57

N-SF14

N-LASF9N-SF2SF2*

SF5N-LAF7N-LASF45

N-F2

LLF1

N-BAF51

N-BAF4

N-BAF52

N-BAF10

N-FK51A*

N-PK51*N-PK52A

N-SF66

SF4

P-SF68

P-SK58A

N-LASF43P-LASF50P-LASF51

P-LAK35P-SK60

P-SF69

P-LAF37

N-LAK33BP-BK7

SF11

SF1LASF35

N-LASF46B

N-LASF46A

Pg,F-DiagramDescription of Symbols

N-glasses

P-glasses

Classical crown and �int glasses

Glasses suitable for precision molding

HT – High transmittance glasses

HTultra – Ultra high transmittance glasses

* Available in step 0.5

Back to index➜ ➜

Refractive Index and Dispersion

Fig. 2: Pg,F as a function of the Abbe number for SCHOTT’s optical glass assortment. Additionally the normal line is given.

TIE-29

5

2.3 Sellmeier Dispersion EquationThe Sellmeier Equation is especially suitable for the progres-sion of refractive index in the wavelength range from the UV through the visible to the IR area (to 2.3 µm). It is derived from the classical dispersion theory and allows the description of the progression of refractive index over the total transmis-sion region with one set of data and to calculate accurate intermediate values.

n2(λ) – 1 = B1 · λ2

+ B2 · λ2

+ B3 · λ2

(10)(λ2 – C1) (λ2 – C2) (λ2 – C3)

The determination of the coefficients was performed for all glass types on the basis of precision measurements by fitting the dispersion equation to the measurement values. The coefficients are listed in the data sheets.

The dispersion equation is only valid within the spectral region in which refractive indices are listed in the data sheet of each glass. Interpolation is possible within these limits. The wave-lengths used in the equation have to be inserted in µm with the same number of digits as listed in Table 1. For prac tical purposes Equation (10) applies to refractive indices in air at room temperature. The achievable precision of this calculation is generally better than 1 · 10 – 5 in the visible spectral range. The coefficients of the dispersion equation can be reported for individual glass parts upon request. This requires a precision measurement for the entire spectral region, provided the glass shows sufficient transmission.

Back to index➜ ➜

Refractive Index and Dispersion

Wavelength [nm] Designation Spectral Line Used Element

2325.42 infrared mercury line Hg

1970.09 infrared mercury line Hg

1529.582 infrared mercury line Hg

1060.0 neodymium glass laser Nd

1013.98 t infrared mercury line Hg

852.11 s infrared cesium line Cs

706.5188 r red helium line He

656.2725 C red hydrogen line H

643.8469 C' red cadmium line Cd

632.8 helium-neon-gas-laser He-Ne

589.2938 D center of double sodium line Na

587.5618 d yellow helium line He

546.074 e green mercury line Hg

486.1327 F blue hydrogen line H

479.9914 F' blue cadmium line Cd

435.8343 g blue mercury line Hg

404.6561 h violet mercury line Hg

365.0146 i ultraviolet mercury line Hg

334.1478 ultraviolet mercury line Hg

312.5663 ultraviolet mercury line Hg

296.7278 ultraviolet mercury line Hg

280.4 ultraviolet mercury line Hg

248.3 ultraviolet mercury line Hg

Tab. 1: Wavelengths for a section of frequently used spectral lines.

TIE-29

6

Temperature [ºC]

N-BK7 SF57 N-PK51 N-LAF2 F2

-100 -80 -60 -40 -20 0 20 40 60 80 100 120 140

15

10

5

0

-5

-10

-15

temperature [ºC]

∆n

rel[1

0-4]

N-BK7 SF57 N-PK51 N-LAF2 F2

-100 -80 -60 -40 -20 0 20 40 60 80 100 120 140

15

10

5

0

-5

-10

-15

∆n

rel [

10-4]

3. Temperature Dependence of Refractive Index

The refractive index of glass is not only dependent on wavelength, but also on temperature. The relationship of refractive index change to temperature change is called the temperature coefficient of refractive index. This can be a positive or a negative value. The data sheets contain infor-mation on the temperature coefficients of refractive index for several temperature ranges and wavelengths. The temperature coefficients of the relative refractive indices Δnrel/ΔT apply for an air pressure of 0.10133 · 106 Pa. The coefficients of the absolute refractive indices dnabs/dT apply for vacuum.

The temperature coefficients of the absolute refractive indices can be calculated for other temperatures and wavelengths values with the aid of Equation (11).

Definitions: T0 Reference temperature (20 °C) T Temperature (in °C) ΔT Temperature difference versus T0

λ Wavelength of the electromagnetic wave in a vacuum (in µm)

D0, D1, D2, E0, E1 and λTK: constants depending on glass type

The constants of this formula given in the glass data sheet in general are valid for a temperature range from –100 °C to +140 °C and a wavelength range from 0.3650 µm to 1.014 µm. The temperature coefficients in the data sheets are guideline values.

Upon request, measurements can be performed on individual melts in the temperature range from –100 °C to +140 °C and in the wavelength range from 0.365 µm to 1.014 µm with a precision better than ± 5 · 10 – 7/K. The constants of the disper-sion formula are also calculated from the measurement data and listed on the test certificate.

dnabs(λ,T)=n2 (λ,T0) – 1 · (D0 + 2 · D1 · ΔT + 3 · D2 dT 2 · n(λ,T0)

· ΔT2 +E0 + 2 · E1 · ΔT

) (11)λ2 – λ22

K

The temperature coefficients of the relative refractive indices Δnrel/ΔT and the values for Δnabs can be calculated with the help of the equations listed in Technical Information TIE 19.

Figure 3 shows the absolute temperature coefficient of refractive index for different glasses, temperatures and wavelengths.

Back to index➜ ➜

Refractive Index and Dispersion

Fig. 3 : Change of the relative refractive index (catalog value at 20 °C) with temperature of some different glass types as shown in TIE-19.

TIE-29

7

4. Influence of the Fine Annealing Process on the Refractive Index and Abbe number

The optical data for a glass type are chiefly determined by the chemical composition and thermal treatment of the melt. The annealing rate in the transformation range of the glass can be used to influence the refractive index within certain limits (depending on the glass type and the allowable stress birefrin-gence). Basically slower annealing rates yield higher refractive indices. In practice, the following formula has proven itself.

nd(hx) = nd(h0) + mnd · log(hx/h0) (12) h0 Original annealing ratehx New annealing ratemnd Annealing coefficient for the refractive index

depending on the glass type

An analogous formula applies to the Abbe number.

nd(hx) = nd(h0) + mnd · log(hx/h0) (13)

mnd Annealing coefficient for the Abbe number

depending on the glass type

The annealing coefficient mvd can be calculated with the

following equation:

mnd = (mnd – nd [h0] · mnF – nC ) / ((nF – nC) + 2

· mnF – nC · log (hx/h0)) (14)

The coefficient mnF – nC has to be determined experimentally.

The refractive index and Abbe number dependence on annealing rate is graphically shown in Figure 4.

Back to index➜ ➜

Refractive Index and Dispersion

Fig. 4 : Dependence of refractive index nd (a: upper) and Abbe number nd (b: lower) on the annealing rate for several glass types. Reference annealing rate is 2 °C/h [3].

Figure 4b shows that individual glass types vary greatly in their dependence of the Abbe number on the annealing rate. In general also the Abbe number increases with decreasing annealing rate. High index lead free glass types such as N-SF5 show anomalous behavior. Anomalous behavior means that the Abbe number decreases with decreasing annealing rate.

∆n

d [

10–5

]Annealing rate [ºC/h]

300

200

100

0

–1000.1 1 10

N-BK7

N-KZFS4

N-SF5

SF2

∆v d

[%

]

Annealing rate [ºC/h]

0.3

0.0

–0.3

–0.60.1 1 10

N-BK7

N-SF5

SF2

N-KZFS4

∆n

d [

10–5

]

Annealing rate [ºC/h]

300

200

100

0

–1000.1 1 10

N-BK7

N-KZFS4

N-SF5

SF2

∆v d

[%

]

Annealing rate [ºC/h]

0.3

0.0

–0.3

–0.60.1 1 10

N-BK7

N-SF5

SF2

N-KZFS4

TIE-29

8

∆nd [10 –5]

∆v d

[%

]

– 100 – 80 – 60 – 40 – 20 0 20 40 60 80 100

0.6

0.4

0.2

0.0

– 0.2

– 0.4

– 0.6

glass for pressing

glass for �ne annealing

10 8 6 41 0.60.8

0.10.2

0.40.60.814680

2°C/h

2°C/h

Step 3

Step 2

Step 1

Step 0.5

Values for a annealing coefficients of some optical glasses are shown in Table 2. We will provide the values for the annealing coefficients of our glasses upon request.

mnd mnF–nc mnd

SCHOTT N-BK7® – 0.00087 – 0.000005 – 0.0682

SF2 – 0.00056 0.000013 – 0.0523

N-SF5 – 0.00242 – 0.000182 0.1654

Back to index➜ ➜

Refractive Index and Dispersion

for a given glass part can be adjusted by a fine annealing step along this characteristic line.

Glass for cold processing has to be fine annealed to reduce internal stresses. During this fine annealing the annealing rate is in general lower than 2 °C/h. The initial refractive index has to be adjusted during melting in such a way that the desired tolerances can be reached during fine annealing. The initial refractive index of SCHOTT N-BK7® for example is in general lower than the target value.

Glass for hot processing i.e reheat pressing is subjected to much more rapid annealing. The heat treatment processes used by the customer in general use annealing rates much higher than 2 °C/h. Therefore for SCHOTT N-BK7® pressings for example the initial refractive index needs to be higher than the target value. We deliver an annealing schedule for each batch of glass for hot processing purpose. This annealing schedule contains the initial refractive index at 2 °C/h and the limit annealing rates to stay within the tolerances.

The annealing rate can be used to adjust the refractive index and Abbe number to the desired tolerance range.

In practice the annealing rate influences the refractive index and the Abbe number simultaneously. Figure 5 shows a diagram of the Abbe number versus the refractive index for SCHOTT N-BK7®. The rectangular boxes indicate the toler-ance limits (steps) for the refractive index and the Abbe num-ber. For example the largest box indicates the tolerance bor-ders for step 3 in refractive index and step 3 in Abbe number. The smallest box indicates step 0.5 in refractive index and Abbe number. The center of the frames is defined by the nominal catalog value.

After melting the optical glass is cooled down at a high anneal-ing rate. To control the refractive index during the melting process samples are taken directly from the melt after each casting. These samples are cooled down very fast together with a reference sample of the same glass. The reference sample has a known refractive index at an annealing rate of 2 °C/h. By measuring the change in refractive index of the reference sample the refractive index of the sample can be measured with moderate accuracy in the range of ± 10– 4.

The annealing rate dependence of the Abbe number and refractive index of each glass is represented by a line in the diagram having a slope that is characteristical for the glass type. For a given melt the position of the line in the diagram is given by the initial refractive index/Abbe number measure-ment for a cooling rate of 2 °C/h as a fix-point together with the glass typical slope. The refractive index and Abbe number

Tab. 2: Annealing coefficients for several selected glass types.

Fig. 5: The influence of the annealing rate on the refractive index and Abbe number of SCHOTT N-BK7® for different initial refractive indices.

TIE-29

9

∆n

fro

m c

atal

og

ue v

alue

[10

– 5]

35

30

25

20

15

10

5

0

Batch No.0 5 10 15 20 25

Position of delivery lot =value in test report = (nmax + nmin)/2 (mid-level value of delivered batches)

Variation in delivery lot: e.g. SN < ± 10 · 10

–5 around position mid-level value

refractive index homogeneity within a single piece: e.g. H2 < 2 · 10– 5

Back to index➜ ➜

Refractive Index and Dispersion

5. Tolerances

The refractive indices, which are listed to 5 decimal places in the data sheets, represent values for a melt with nominal nd-nd position for the glass type in question. The refractive index data are exact to five decimal places (for λ > 2 µm: ± 2 · 10 – 5). The accuracy of the data is less in wavelength regions with limited transmission. All data apply to room temperature and normal air pressure (0.10133 · 106 Pa).

Defining tolerances for the refractive index of a glass the customer has to distinguish between the refractive index tolerance, the tolerance of refractive index variation within a lot and the refractive index homogeneity (Figure 6).

All deliveries of fine annealed block glass and fabricated glass are made in lots of single batches. The batch may be a single block or some few strip sections.

The refractive index and Abbe number tolerance is the maxi-mum allowed deviation of a single part within the delivery lot from nominal values given in the data sheets of the catalog. The refractive index of the delivery lot given in the standard test certificates is given by the following formulae:

nlot = (nmax + nmin)/2 (15)

nmax is the maximum and nmin the minimum refractive index within the lot.

Fig. 6: Refractive index variation from within a production sequence.

Tab. 3: Refractive Index Tolerances. * only for selected glass types

The refractive index variation from part to part within a lot is always smaller than ± 5 · 10 – 5. The refractive index homo-geneity within a single part is better than 4 · 10 – 5 ISO 12123 (equivalent to ± 2 · 10 – 5 according ISO 10110) in general. [4; TIE-26] A short summary of the refractive index tolerance, variation and homogeneity grades can be found in table 3. More information is given in the optical glass catalogue [5].

Tolerance Grade Refractive Index [· 10 – 5] Abbe Number

Absolute

Step 3 ± 50 ± 0.5 %

Step 2 ± 30 ± 0.3 %

Step 1 ± 20 ± 0.2 %

Step 0.5* ± 10 ± 0.1 %

Variation

SN ± 10 –

S0 ± 5 –

S1 ± 2 –

Homogeneity ISO 12123 (ISO 10110)

H1 4 (± 2) –

H2 1 (± 0.5) –

H3 0.4 (± 0.2) –

H4 0.2 (± 0.1) –

H5 0.1 (± 0.05) –

TIE-29

10

Back to index➜ ➜

Refractive Index and Dispersion

5.1 Tolerance Step 0.5 [3]SCHOTT is the only manufacturer to offer optical glasses in the new tolerance step 0.5. For step 0.5 the maximum allowed deviation from the nominal values listed in the datasheet is only ± 0.0001 for the refractive index nd and ± 0.1 % for the Abbe number nd. This new tolerance grade can be offered only for selected glass types. Among these glass types are the following glasses: N-FK51A, N-PK51, N-FK5, SCHOTT N-BK7®, N-BK7HT, N-PSK53A, N-SK2, N-KZFS2, N-KZFS4, N-KZFS4HT, N-KZFS5, N-KZFS8, N-KZFS11, N-LAK9, N-LASF44, SF2, SF57HTUltra and N-SF5. The list comprises glass types, which are especially important for best color correction such as FK-, PK- and KZFS-types and which are often required in narrowest possible tolerances. Even though SCHOTT commits itself to be capable to deliver tolerance step 0.5 for the range of the listed

5.2 Tolerance of the refractive index of optical glasses in

the near IR

The question often arises if the tolerances for the refractive index at standard wavelength d can be transferred to longer wavelengths in the spectrum. This is approximately sure for wavelengths within the visible spectral range, whereas for wavelengths in the near IR range up to 1.7 µm one has to look a little bit more closely on the variation of the dispersion for different melts of different glass types. A first evaluation was published in [6], comparing extrapolations from v-block meas-urements in the visible to the IR range with precision spec-trometer measurements (URIS). Glas types evaluated were SCHOTT N-BK7®, N-KZFS4, N-PK51, N-PK52A, N-SF6, SF57, N-LAK22, N-LASF31A, F2 and N-SF57.

The phenomenology of dispersion curves and the comparison of predicted with measured refractive index curves in the near infrared wavelength range lead to the following observations,

glass types, it is possible that other glass types are available also in the narrowest tolerances. This will be checked on request. The fine annealing process has to be done with furnaces with spe-cial precision temperature control and high temperature field homogeneity. Therefore step 0.5 glasses are available as fine annealed cut blanks and most of the glass types are also avail-able as reheat pressings. All Step 0.5 tolerance grades are verified using the v-block with enhanced accuracy measurement procedure. For glasses with low dispersion (high Abbe number) like N-FK51A and N-PK51 the v-block contains an additional reference samples measured to an accuracy of ± 0.4 · 10 – 5 with the prism spec-trometer (compare table 4).

• Melts with refractive index values very close to each other in the visible light range may have significant deviations in the near infrared wave length range. Slope and curvature can differ among melts and also with respect to the catalog curve.

• Extrapolations from test certificate data obtained in the visible light range improved by using catalog relative partial dispersion data can lead to deviations from real measured values up to ± 5 · 10 – 5 or in some cases even more above 1.7 µm wavelength.

• Using Abbe number nd, defined for the directly neighboring IR range with the spectral lines C, t and s deviations of extrapolated dispersion curves reduce roughly by a factor of two above 1.7 µm.

• For better extrapolation it is recommended to perform a v-block measurement with enhanced accuracy because of its extended wavelength range.

TIE-29

11

Back to index➜ ➜

Refractive Index and Dispersion

6. Refractive Index Measurement

For refractive index measurement two different measurement setups are used: the v-block refractometer and the spectral goniometer. Figure 7 shows the principle of the v-block measurement. The samples are shaped in a nearly square shape. One sample is about 20 x 20 x 5 mm small. The sample will be placed in a v shaped block prism. The refractive index of this prism is known very precisely. The refraction of an in -coming light beam depends on the refractive index difference between the sample and the v-block-prism. The advantage of this method is that up to 10 samples can be glued together into one v-block stack. Therefore many samples can be meas-ured in a very short time. The relative measurement accuracy is very high therefore differences in refractive index within one v-block stack can be measured very accurately. Standard measurement temperature is 22 °C.

The spectral goniometric method is based on the measure-ment of the angle of minimum refraction in a prism shaped sample. This is the most accurate absolute refractive index measurement method. In our laboratory we use an automated spectral goniometer with high accuracy and the ability to measure in the infrared and UV region (Figure 8).

With the automated spectral goniometer, the Ultraviolett to infrared Refractive Index measurement System (URIS), the refractive index of optical glasses can be measured to an accuracy of ± 0.4 · 10 – 5. The measurement accuracy for the dispersion (nF-nC) is ± 2 · 10 – 6. These measurement accuracies can be achieved independent of the glass type and over the complete wavelength range from 185 nm to 2325 nm. The measurement is based on the minimum angle of refraction principle. The samples are prism shaped with dimensions of about 35 x 35 x 25 mm3. The standard measurement tem-perature is 22 °C. The temperature can be varied between 18 to 28 °C on request. The standard measurement atmosphere is air. On special request also nitrogen is possible.

Fig. 7: V-block refractormeter principle.

Fig. 8: Automated spectral goniometer.

Immersion oil

nairnair

θnV – block

nsample

Incident light ray at wavelength λ

Optical axis

Sample with higherrefractive index

Sample with lowerrefractive index

Sample

V-Block-Prism with precisely known

index of refraction

TIE-29

12

Hattenbergstrasse 10 55122 Mainz

Germany Phone +49 (0)6131/66-1812 Fax +49 (0)3641/2888-9047

[email protected]

7. Literature

[1] The properties of optical glass H. Bach & N. Neuroth (Editors), Springer Verlag 1998

[2] Temperature Coefficient of the Refractive Index SCHOTT Technical Information TIE-19

[3] Optical glass with tightest refractive index and disper-sion tolerances for high-end optical designs, Ralf Jedamzik, Steffen Reichel, Peter Hartmann, SPIE Proceeding 8982-51, (2014)

[4] Homogeneity of Optical Glass SCHOTT Technical Information TIE-26

[5] SCHOTT Optical Glass Pocket Catalogue

[6] Optical glass: dispersion in the near infrared Peter Hartmann, SPIE Proceedings Vol. 8167, (2011)

[7] V-Block refractometer for monitoring the production of optical glasses, U. Petzold, R. Jedamzik, P. Hartmann, and S. Reichel, Proc. SPIE 9628, (2015)

Table 4 shows a summary of the refractive index measure-ments available at SCHOTT.

The temperature coefficient of refractive index is measured using the automated spectral goniometer and a temperature controlled climate chamber with a temperature range from –100 °C up to +140 °C. The temperature coefficient can be measured with an accuracy of ± 5 · 10 –7/K.

With the introduction of step 0.5 tolerances also for low dis-persion glasses the question arises how accurate is the Abbe number measurement with the v-Block refractometer. Figure 9 shows the results of reproducibility measurement for the glass types N-FK58 and SF57. The plot shows the distribution of the nd and nd of SF57 (blue tilted crosses) and N-FK58 (green standing crosses) determined by V-block refractometer. The filled red signs correspond to the center of the V-block refrac-tometer measurements (SF57: circle and N-FK58: square). The average of several SCHOTT’s spectral goniometer URIS

measurements (SF57: black diamants and N-FK58 orange circles) of the same piece of glass defines the origin of the plot. To give an impression of the deviation size the tolerance range of SCHOTT’s best commercially available quality step 0.5 (red dashed line) is added.

The standard deviations of the V-block measurements of N-FK58 (SF57 respectively) are 0.2 · 10 – 5 (1.1 · 10 – 5) for the refractive index and 0.017 % (0.008 %) for the Abbe number. Systematic deviations can be corrected by implementing an URIS sample to the v-block stack. In the given example the systematic deviations are – 1.8 · 10 – 5 (0.2 · 10 – 5) for the refrac-tive index and – 0.011% (– 0.01 %) for the Abbe number of N-FK58 (SF57 respectively) [7].

Back to index➜

Refractive Index and Dispersion

MeasurementMeasurement accuracy

Wavelengths MethodRefractive

indexDispersion

V-block standard

± 3 · 10 – 5 ± 2 · 10 – 5 g, F', F, e, d, C', C v-block

refractometerV-block enhanced

± 2 · 10 – 5 ± 1 · 10 – 5 i, h, g, F', F, e, d, C', C, r, t

Precision spectrometer

± 0.4 · 10 – 5 ± 0.2 · 10 – 7 185 nm – 2325 nm

URIS auto-matic spectral goniometer

Tab. 4: Absolute refractive index measurement accuracies.

Fig.9: Reproducibility of V-block refractometer. Red box indicates the toler-ance step. In order to give an impression of the deviation size we added the tolerance range of SCHOTT’s best commercially available quality step 0.5 (red dashed line).

TIE-29

Vers

ion

Ap

ril 2

016

| SC

HO

TT A

dvan

ced

Op

tics

rese

rves

the

rig

ht t

o m

ake

spec

ifica

tion

chan

ges

in t

his

pro

duct

flye

r w

ithou

t no

tice.

Recommended